Graphene, owing to its unique chemical structure and extraordinary chemical, electrical, thermal, optical, and mechanical properties, has opened up a new vista of applications, specifically as novel sensing platforms. The last decade has seen an extensive exploration of graphene and graphene-based materials either alone or modified with nanoparticles and polymers for the fabrication of nanoscale biosensors. These biosensors displayed excellent conductivity, high sensitivity, and selectivity, good accuracy, and precision, rapid detection with low detection limits as well as long-term stability. The unmatched properties of graphene and graphene-based materials have been applied for the detection of a number of chemical and biological molecules successfully for the diagnosis of a variety of diseases, pathogens, and biomarkers of the diseases. This review is aimed to cover the fabrication methods, functionalization techniques, and biomedical applications along with the recent advancements in the field of development of graphene-based biosensors. Recent clinical trials and patents as well as market trends and opportunities associated with graphene-based biosensors are also summarized. The application of graphene-based biosensors in the detection of SARS-CoV-2 causing COVID-19 is also reviewed.
Diagnosis of diseases and their biomarkers requires accurate and highly sensitive methods and to achieve it, a number of conventional and novel methods are available [1,2]. Conventional methods include polymerase chain reaction, lateral flow immunoassay, electrochemical methods, DNA sequencing and microarrays and fluorescence microarray, and enzyme-linked immunosorbent assay (ELISA) techniques [3,4]. These techniques however require highly precise instruments, costly reagents, complicated sample preparation steps, and tedious quantification methods in order to achieve accurate and sensitive detection [5,6]. In addition, these techniques have limitations when it comes to detecting the disease in real-time. Novel methods include the use of sensors that are comparatively inexpensive, simple, and highly specific techniques for the detection of target biomolecules. These sensors can be used in real-time to monitor and diagnose diseases and therefore have broad clinical applications [7,8,9,10]. The added advantages associated with sensors are their use in detecting the diseases at an early stage and requires minimal invasive methods.
These sensors are fabricated using nanomaterials that further improve their chemical and electrical properties and therefore their sensitivity . A number of nanomaterials are being used to fabricate these sensors, and graphene and graphene-based nanomaterials have shown exceptional properties with enhanced signal detection [11,12,13]. Graphene-based nanomaterials also support the incorporation of a number of biological molecules such as proteins, enzymes, antibodies, DNA, and cells owing to their excellent biocompatibility with these molecules . Sensors immobilized with biological molecules are called biosensors and are used in the detection of various molecules and cells [14,15].
Graphene, first discovered in 2004, is a carbon-based nanomaterial arranged in form of a single layer of sp2 carbon sheet having atoms arranged in a honeycomb lattice [16,17]. It possesses a number of unique properties including high intrinsic mobility, unequaled flexibility, large surface area, and excellent electronic transportation capabilities. The two-dimensional structure of graphene allows its functionalization with a number of linker molecules making it a highly sensitive and selective candidate for biosensing applications [18,19,20]. Graphene is available in a number of forms and each form has its own properties and applications. These forms include the few-layer graphene, multilayer graphene, graphene oxide (GO), reduced graphene oxide (rGO), and graphene nanoplatelets (GNP), of which GO and rGO are used for biosensing applications [21,22,23,24,25,26,27].
Apart from the biological applications, graphene-based sensors are also used in nonmedical fields including nanoelectronics, optoelectronics, nanocomposites, supercapacitors, field-effect transistors (FET), solar cells, pH sensors as well as gas sensors [28,29,30]. Graphene offers ultrahigh loading capacity for the biomolecules and drugs along with strong adsorptive capabilities and high mechanical strength, making it one of the most widely used nanomaterials for the development of biosensors. Since every atom of graphene is present on the surface, the molecular interaction and transportation of electrons from the adsorbed molecules through graphene are easy [31,32] and result in the ultrasensitive detection of biomolecules. Graphene-based biosensors have opened up new vistas for the early diagnosis of a number of life-threatening conditions and severe diseases along with real-time health monitoring. For instance, several graphene biosensors showed a successful diagnosis of various cancer forms and cardiovascular diseases by detecting their biomarkers. Real-time monitoring of disease would help change the quality of life of the patients, and the graphene-based electrochemical biosensors showed immense potential for implantable devices that would detect the biomarkers in real-time assessing the severity of the disease.
In this review, the development of graphene-based biosensors with their biomedical applications is discussed. The fabrication and immobilization methods used in the development of graphene-based biosensors are reviewed. Recent studies concerning graphene-based biosensors including the application in the COVID-19 testing along with the clinical trials and patents are also summarized.
2 Development of graphene-based biosensors
2.1 Fabrication methods
There exists an industrial revolution with respect to graphene and its utilization into several products around us including drugs and their delivery, medical devices, as well as many products and devices that improve the quality of life. Generally, graphene is produced using two main strategies and each strategy includes different fabrication methods. In a top-down strategy, graphene derivatives can be obtained from any carbon source such as graphite flakes or powder that is exfoliated mechanically or electrochemically and is subjected to chemical oxidation–reduction reactions. For instance, scotch tape techniques, sonication in a liquid phase, Hummers method, Brodie methods, etc., are the top-down techniques used in the fabrication of graphene derivatives. In contrast, the bottom-up strategy depends on the synthesis of graphene layers from the carbon atom bases and involves numerous fabrication methods such as chemical vapor deposition, epitaxial growth, thermal pyrolysis, etc. All these fabrication techniques have their own advantages and disadvantages [33,34,35,36,37]. Fabrication is a critical step in the development of graphene-based biosensors as it can influence the nature of graphene. Graphene and its derivatives are known to be excellent supporting materials that have been exploited extensively in the development of biosensors. A typical biosensor consists of two layers of receptors and transducers that are attached to each other, as shown in Figure 1.
The upper layer is made of receptors that are composed of biomolecules such as enzymes, proteins, DNA, or antibodies with specific biorecognition to the targeted analytes. These receptor molecules that are attached to the transducer layer are very sensitive to physicochemical changes upon biomolecular interactions and are capable to convert them into measurable signals [38,39,40]. Herein, graphene and its derivatives work as transducers for these signals that can be detected electrochemically, optically, or thermally. Therefore, graphene-based biosensors are fabricated according to the detection technique, and electrochemical biosensors are more commonly employed in comparison to optical biosensors [41,42].
In the electrochemical biosensors, the designed sensors usually consist of a three-electrode system: working electrode, counter electrode also known as the auxiliary electrode, and the reference electrode. These electrodes are coated with graphene-based nanomaterials using fabrication methodologies including coating, direct growth methods, direct deposition methods, and printing-based methods. Direct coating is the most commonly employed technique for the fabrication of biosensors due to its simplicity, cost-effectiveness, and it does not require any specific instrument . Usually, a solution/gel containing graphene or graphene derivatives is used to coat the surface of electrodes using methods such as drop-casting, dip coating, spin coating, and blade coating. Each coating technique has its advantages and disadvantages, and therefore, the choice of the technique depends on the desired film properties such as thickness, uniformity, and surface area. Generally, the direct coating method is the first choice for biosensors; however, it involves multistep fabrication, material wasting, and is a time-consuming process [43,44,45,46,47]. Direct deposition-based methods involve direct deposition of graphene and other nanomaterials on the electrode surface by dipping the electrodes in a solution containing graphene and applying an electrical voltage to control the coating. The electrospinning technique involves the spinning of a nozzle jet containing the graphene nanomaterial onto the electrode surface. The electrospray deposition method is similar to electrospinning deposition; however, it offers control of droplet size, charge, and speed, and therefore, is utilized in industrial-scale fabrication with high precision [48,49,50,51].
Subsequently, printing-based fabrication methods were introduced with the revolution of 3D printers. Printing techniques are very attractive because of many reasons including large-scale fabrication, are cost-saving, and require low temperatures and solution ink. These methods fit properly with graphene-based biosensors and therefore are exploited extensively in the development of various biosensors [52,53,54,55]. In this method, the ink solution is prepared and sprayed using various techniques including screen-printing, inkjet printing, nozzle-jet printing, and laser scribing printing. Generally, these printing techniques are similar to each other in principle with small variations; for instance, screen printing is used for a thicker nanofilm and is commonly employed for industrial-scale fabrication due to its simplicity and utilization of prefabricated mesh-covered frames to allow the transfer of the desired pattern to the electrode surface. Direct spay of ink solution can be achieved using inkjet printing that exhibits more controlled drop size and high-resolution pattern, while nozzle-jet printing is similar to inkjet printing with the addition of external pressure. Therefore, nozzle-jet printing is suitable for more viscous ink solutions. Meanwhile, laser scribing printing is an advanced technique with high fabrication flexibility for many substrates and supporting materials as well as small size sensors. However, printing using instrumental techniques require special handling skills and need preparation of ink solution critically.
Another method of fabrication of biosensors is the direct growth of nanomaterials on the surface of electrodes. This method gained more attention recently due to several controllable parameters during fabrication such as time, temperature, pH, pressure, and concentration. This strategy depends on the recruitment of several experimental environments to catalyze the nanomaterial growth on the electrode surface via numerous techniques such as thermal, hydrothermal decomposition, anodization, and chemical decomposition [56,57]. However, limited attention to these methods is given for the fabrication of graphene-based biosensors as it involves limited direct growth to the electrode surface.
2.2 Functionalization methods
Due to its unique electro- and thermomechanical properties, applications of graphene are practically limitless. It showed excellent potential in transforming many areas ranging from electronics to healthcare such as touch screens, sensors, biofunctionalized graphene, quantum dots, novel drug delivery, nanodevices for DNA sequencing, etc. . The unique molecular structure of graphene characterized by sp2-hybridized carbons, large specific-surface area (2,630 m2 g−1) as well as strong van der Waal cohesive forces render graphene to agglomerate easily and prevent its uniform dispersion . Moreover, graphene sheets have poor water solubility because of the strong π–π interactions between the sheets . To address this, the functionalization of graphene is performed in order to redesign its electronic, physical, and chemical properties . To date, functionalization is the only effective technique that helps in reducing the cohesive forces between graphene sheets and thus prevents its agglomeration without losing its inherent properties .
Functionalization involves the process of adding new functions, characteristics, potentials, or properties to graphene by changing its surface chemistry . Functionalization modifies inert graphene sheets and is exceptionally effective in fabricating sensors that have huge biomedical, electrochemical, and diagnostic applications . Functionalization of pristine graphene through the covalent and noncovalent functionalization provides a multitude of chemically activated, soluble, hybrid graphene  surfaces. Covalent functionalization forms a stable covalent bond, whereas the noncovalent functionalization is formed through hydrogen bonds, π–π interactions, and van der Waals interactions .
2.2.1 Covalent functionalization
Covalent functionalization of graphene involves rehybridization of sp2 C-atoms into the sp3-hybridized tetrahedral configuration, chiefly at the edge . This process of covalent surface modifications is also known as chemisorption (grafting) of molecules on graphene lattice . This rehybridization of the π-conjugated carbon network often forms hybrid-graphene materials with chromophores or polymers that enhance the dispersibility of graphene . Figure 2 illustrates different covalent functionalization techniques employed in the development of graphene-based biosensors.
188.8.131.52 Free radical addition (FRA)
Free radicals are extremely reactive uncharged chemical species that contain an unpaired electron. They can react readily with the compounds containing multiple bonds to produce another radical, which reacts further and goes on . FRA can be achieved through one or more synthetic approaches such as aryl diazonium salts , peroxides, Bergman cyclization , and the Kolbe–Schmitt reaction . Among these, aryl diazonium salts are the most studied method for stabilizing graphene layer with enormous applications in the development of semiconducting nanomaterials, atom transfer radical polymerization, coupling reactions through click chemistry, grafting of heterostructures, and tuning of electrical conductivity . The delocalized π-electrons of the graphene cage are shifted to electron-deficient diazonium electrophile and eliminate its N2 molecule thereby forming a highly reactive aryl free radical that eventually reacts with the carbon atom of the graphene lattice and forms a covalent bond . Functionalization through benzoyl peroxide (BPO) is another common approach for the FRA. BPO has been widely utilized as an important organic peroxide initiator because of its easily accessible benzoyloxy radicals after homolytic fission [76,77]. The functionalization of graphene by Bergman cyclization has many advantages including simple steps, superior efficacy, tailored structure, and catalyst-free procedure .
184.108.40.206 Nucleophilic addition
The nucleophilic addition reaction is widely employed in the functionalization of pristine graphene sheets due to its electron acceptor properties . Recently, a soluble charm-bracelet-type poly-(N-vinylcarbazole) functionalized graphene sheet has been developed by the reaction of carbanion intermediate of poly(N-vinylcarbazole) and graphene . In another study, covalent modification of rGO was performed through the nucleophilic addition reaction using nitrogen anions, formed by sodium hydride. The π–π interaction and “polymer wrapping” effect between the polymers and graphene resulted in improved dispersion of graphene .
220.127.116.11 Cycloaddition reaction
The cycloaddition reaction involves the formation of a new ring by the σ bonds through the reaction of two π-electron systems . The aromatic properties of graphene is exploited through a number of cycloaddition reactions involving 1,3 dipolar cycloadditions, [2 + 2] cycloadditions, [2 + 1] cycloadditions, and Diels–Alder reaction [83,84,85,86]. Diels–Alder reaction is one of the promising methods for the modification of pristine graphene because of its click-type procedure, high efficiency, versatility, and efficiency . Dihydronaphthalene-grafted graphene was designed using cis-diene and the resulting modified graphene showed a p-type doping effect with improved conductivity that can be used for making transparent electrodes .
18.104.22.168 Electrophilic substitution reactions (ESRs)
Electrophilic aromatic substitution reactions are very fascinating versatile organic reactions where an electrophile substitutes the atom attached to the aromatic ring; usually, a hydrogen atom is replaced by an electrophile . This reaction has gained much attention in the field of covalent functionalization of graphene because ESR can introduce a wide range of functional groups on the graphene surface and thus is a useful tool for tailoring the graphene properties . Some of the hitherto reported ESR functionalization includes halogenation , nitration , sulfonation , Friedel–Crafts acylation, alkylation  reactions, etc.
22.214.171.124 Addition of chromophores
Organic compounds having extended π-system such as porphyrins , phthalocyanines , azobenzenes , and other chromophores were identified as potential candidates for preparing hybrid graphene nanoplates with the superior optical limiting property. Covalently functionalized soluble hybrid porphyrin–graphene was prepared by the reaction of 5-4(aminophenyl)-10,15,20-triphenyl porphyrin and GO in N,N-dimethylformamide (DMF). The amide linkage in the hybrid porphyrin–graphene significantly improved the dispersion and thereby solubility of graphene in organic solvents. Moreover, this donor–acceptor nanohybrid also exhibited superior optical limiting performance due to photoinduced electron and/or energy transfer . Table 1 summarizes different covalent functionalization methods used in the development of graphene-based biosensors.
|S.No.||Types of covalent functionalization||Reaction condition/reagents||Applications||Disadvantages||References|
|1||Aryl diazonium salts||Aryl diazonium molecules||Atom transfer radical polymerization, voltammetric immunosensor, antistatic coatings electrode, supercapacitor, photoactive graphene sheet, nanocomposites||Self-polymerization|||
|2||BPO||Ar-ion laser beam||The electrical conductivity of graphene decreased and the hole-doping level increased||Localized functionalization and a low efficiency||[76,77]|
|3||Bergman cyclization||Enediyne||Carbon-rich nanoparticles/networks, carbon nanomembranes, and nanodevices||High temperature required that is often incompatible with organic substrates|||
|4||Nucleophilic addition||Nucleophile and base||Photonic and optoelectronic devices||Variations in the reactivity of polymers and their dispersion stability|||
|5||Diels–Alder reaction||cis-Diene||p-Type doping effect and improved conductivity to graphene, transparent electrodes||—||[83,84]|
|6||Friedel–Crafts reaction||Methylbenzene, chlorobenzene, or polystyrene||In the preparation of graphene–polymer interface||Polyalkylated products are formed|||
|7||Addition of chromophores||Amine-functionalized prophyrin (TPP-NH2), DMF||Solar-energy conversion materials for optoelectronic devices||—|||
2.2.2 Noncovalent functionalization
Noncovalent interactions are reversible interactions between the graphene and organic molecules or polymers without disruption of the delocalized π-system of graphene and therefore its electronic properties . Physical forces such as hydrophobic, van der Waals, and electrostatic forces are the major forms of interactions utilized in the noncovalent functionalization . Numerous studies reported the immobilization of proteins, DNA–protein complexes, enzyme–drug complexes, functional nanomaterials, and organic supramolecules using a noncovalent functionalization technique . In recent years, enormous advancements were made in terms of functionalization of graphene through π–π stacking with polyaromatic compounds such as naphthalene , pyrene, 4-n-octyl-4′-cyanobiphenyl, tetrafluoro-tetracyanoquinodimethane , 3,4,9,10-perylenetetracarboxylic diimidebisbenzenesulfonic acid , pyridinium-functionalized porphyrin,  etc. Noncovalent immobilization of enzymes on graphene surfaces was also reported to have improved biocatalytic efficiency; for instance, immobilization of glucose oxidase and glucoamylase enzyme for one-pot conversion of starch into gluconic acid . Highly stable and water-soluble gold nanoparticles (Au-NPs) of DNA-decorated graphene nanosheets were also reported to be a promising approach to design a 2D-conductance device for DNA sequencing (Figure 3) .
3 Biomedical applications of graphene-based biosensors
Traditional sensing methods are expensive, require high-precision equipment and costly reagents, and the majority of reactions are not quantifiable in real-time. Graphene-based sensors are now being used as an alternative method for the identification of disease-related biomolecules and they offer a wide range of biomedical applications. Graphene biosensors are easy-to-use, cost-effective, nontoxic, and are equipped with excellent sensing properties . Generally, a sensor consists of two elements: receptor (linked with target molecule) and transducer (converts chemical information into signals). A graphene or GO-based biosensor acts as a transducer converting the receptor–target molecule interaction into a detectable signal. Bioreceptors such as antibodies, enzymes, or nucleic acid are usually immobilized to the transducers in order to allow target molecules to interact (Figure 4) [12,109].
3.1 Detection of microbes
Antibodies, nucleic acids, proteins, and enzymes are immobilized to graphene biosensors using various processes, which can be identified using spectroscopic methods . Attachment of antibodies to the graphene surface is mainly applied for the detection of infectious diseases caused by viruses and bacteria. Table 2 summarizes the studies on graphene-based biosensors used for the detection of microbes including bacteria and viruses. Graphene biosensors have been successfully applied for the detection of Ebola virus [110,111], Escherichia coli , and Zika virus , whereas graphene biosensors modified with silver and gold nanoparticles were developed for the detection of Salmonella typhimurium , hepatitis-C virus (HCV) [115,116], and avian influenza virus H7 . Modifications of graphene biosensors have further been proven to be effective in the detection of diseases as dendrimers, polymers, and cyclodextrin modifications could all be used to diagnose celiac disease , human immunodeficiency virus (HIV) [119,120], and cholera toxin .
|Target||Immunosensor design||Detection methods||Detection limit||Refs|
|Ebola virus||rGO||Electrochemical||2.4 pg mL−1 and 1 μg mL−1||[110,111]|
|E. coli||rGO||Electrical||103 CFU mL−1|||
|Zika virus||Graphene||Electrical||0.45 nM|||
|S. typhimurium||GO–AgNPs nanocomposite||Cyclic voltammetry (CV)||10 CFU mL−1|||
|Hepatitis C virus (HCV)||rGO, rGO/CuNPs||Optical, electrochemical||10 fM, 0.4 nM||[115,116]|
|Influenza A virus||Graphene oxide–MB–chitosan||Electrochemical||9.4 and 8.3 pM|||
|Celiac disease||GQDs on AuNPs with polyamidoamine dendrimer embedded on MWCNTs||Electrochemical||0.1 fg per 6 µL|||
|HIV||G/CVD, GO/PANi||Electrochemical||0.1 ng mL−1, 100 aM||[119,120]|
|Cholera toxin||Graphene–polypyrrole||Surface plasmon resonance||4 pg mL−1|||
|Dengue virus||rGO, rGO/PAMAM||Optical||0.08 pM||[122,123]|
|Rotavirus||GO||Photoluminescence||105 PFU mL−1|||
|Hepatitis B virus||rGO/AuNPs, Gquantum dots||Electrochemical||3.8 ng mL−1, 1 nM||[125,126]|
|Adenovirus||Graphene quantum dots||Optoelectronic||8.75 PFU mL−1|||
|Human papillomavirus (HPV)||MWCNT-NH2-IL-rGO||Electrochemical||1.3 nM|||
|HCV||Magnetic rGO–CuNCs||Electrochemical||405.0 pM|||
|E. coli O157||APTMS–ZnO/c-GO||Electrochemical||0.1 fM|||
|B. anthracis||GO||Fluorescence||0.625 µM|||
|S. aureus||Graphene–AuNPs||Surface acoustic wave||12.4 pg mL−1|||
|Porcine epidemic diarrhea virus||AuNP–MoS2–rGO||Electrochemical||—|||
|E. coli O157||AuNPs–Graphene||Electrochemical||102 CFU mL−1|||
|E. coli K12||AuNPs–Graphene||Electrochemical||12 CFU mL−1|||
Different types of antibodies are immobilized on the graphene surface and are being used for the detection of target molecules. For instance, PAC1 is used for the diagnosis of cardiovascular diseases, anti-GHRL and anti-PYY antibodies for hormone detection, an anti-tTG antibody for celiac diseases, an anti-HCV antibody for Hepatitis C virus, anti-CT for cholera toxin, anti-rotavirus antibodies for rotavirus detection, monoclonal antibodies (H5N1, H1N1, H7) for avian influenza virus H7 and influenza A virus, anti-Zika NS1 antibody for Zika virus, anti-S. typhimurium antibody for S. typhimurium bacteria, and anti-E. coli O157:H7 antibody for the detection of E. coli. Moreover, the Dengue virus and rotavirus have also been identified using antibodies immobilized to GO biosensors [122–124]. Rotavirus and G2 monoclonal antibodies were used in these techniques that bind to the graphene nanomaterial using a carbodiimide-assisted amidation reaction and an electrostatic bond. Another promising breakthrough was achieved when graphene quantum dots were prepared that were successfully applied for the highly sensitive detection of hepatitis B and adenovirus [125–127].
3.2 Detection of nucleic acids and genes
The DNA-based graphene biosensor helps in the detection of various types of biomarkers (DNA, RNA, small molecules, proteins), viruses, and genes using electrochemical and fluorescent detection techniques (Table 3). In the electrochemical approach, the immobilization of DNA is achieved using covalent bonds, π–π interactions, or EDC/NHS chemistry on the surface of graphene biosensors. Electrochemical signals are generated when DNA is hybridized or oxidized. Differential pulse voltammetry, CV, and electrochemical impedance spectroscopy were used to quantify voltage and current shifts triggered by a number of factors, such as conductivity changes or electron depletion caused by oxidation or hybridization. In the fluorescence approach, the immobilization of DNA can be achieved through π–π interaction (direct adsorption of the DNA probe on the biosensor). This is based on the hybridization of two single-stranded DNA (ssDNA); one strand being fluorescently labeled while the other is the complementary DNA to the target DNA.
|Target||Immunosensor design||Detection methods||Detection limit||Refs|
|Staphylococcus aureus DNA||GO–DNA sensor||Fluorescence detection||0.00625 nM|||
|HIV-1 gene||AuNPs–GO nanocomposite||Fluorescence detection||15 fM|||
|T antigen gene of SV40 DNA||GO||Fluorescence detection||14.3 nM|||
|ssDNA||GO||Fluorescence detection||200 nM and||[139,140]|
|DNA and exonuclease activity||GO ethidium bromide (EB)||Electrochemical detection||32 nM|||
|Amelogenin gene (AMEL)||Glassy carbon electrode modified with rGO (GCE/RGO)||Electrochemical detection||3.2 × 10−21 M|||
|Hepatitis B virus (HBV) gene||Pencil graphite electrode modified with GO (GO/PGE)||Electrochemical detection||2.02 µM|||
|ssDNA||Thionine functionalized rGO (Thi–rGO) and rGO-graphene double-layer electrode||Electrochemical detection||4.28 × 10−19 M and 1.58 × 10−13 M||[144,145]|
|Nucleic acids||Deformed monolayer graphene channel||Electrochemical detection||600 zM and 20 aM|||
|RNA HIV-1 gene||Graphene field-effect transistor biosensor||Electrochemical detection||0.1 fM|||
|HIV-1 gene||Polyaniline/graphene biosensor||Electrochemical detection||1.0 × 10−16 M|||
|miRNA let-7b||Crumpled graphene FET||Electrical||600 zM|||
|DNA hybridization||Armchair graphene nanoribbon-Au electrode- FET||Electrical||—|||
|Nucleic acids||Zirconia reduced graphene oxide–thionine (ZrO2–rGO–Thi)||Electrochemical||24 fM|||
3.3 Detection of enzymes and other molecules
Similarly, a number of enzymes and related biomolecules such as horseradish peroxidase, laccase, glucose, and bilirubin oxidase were also immobilized onto the graphene biosensor via covalent bonding, physical entrapment, 1-ethyl-3-(3-dimethylaminopropyl)carbodiimide hydrochloride/N-hydroxy sulfosuccinimide (EDC/NHS) chemistry, and adsorption methods. These types of sensors are based on two main mechanisms: catalytic properties of the enzymes and enzyme activity inhibition/moderation. Different molecules such as phenols (2,6-dimethozyphenol), hydrogen peroxide, caffeic acid, glucose, bilirubin, and 17β-estradiol have been detected by enzyme-immobilized graphene biosensors (Table 4).
|Target with enzymes||Immunosensor design||Detection methods||Detection limit||Refs|
|17β-Estradiol with laccase||GO–rhodium nanoparticles||Electrochemical detection||0.9–11 pM|||
|Catechol with laccase||Graphene/cellulose microfiber||Amperometric detection||0.085–209.7 µM|||
|Hydrogen peroxide with horseradish peroxidase||3D graphene/methylene blue-carbon nanotubes and calcium carbonate (CaCO3) microspheres encapsulated with graphene capsule||Electrochemical detection||0.2 μM to 1.1 mM and 0.01–12 mM||[153,154]|
|Caffeic acid with laccase||Molybdenum disulfide and graphene quantum dots||Electrochemical detection||0.38–100 μM|||
|Glucose with glucose oxidase||3D graphene and 3D GO and polyanilline||Electrochemical detection||0.3–6 mM and 0.07–1.10 mM||[156,157]|
|l-Lactic acid||Lactate dehydrogenase immobilized on the active graphene surface using Nafion, chitosan, and glutaraldehyde||Electrochemical||7.5 mM|||
|Acetaminophen, Epinephrine, tyrosine||l-Aspartic acid-modified CVD graphene electrode||Electrochemical||0.011, 0.006, 0.31 µM respectively|||
|Lung cancer biomarker (CD59)||GO–NP embodied complex||Electrochemical||1 fg mL−1|||
|Glucose oxidase||CVD-graphene on SiO2/Si substrate followed by deposition of Nafion||Electrochemical||124.19 µM|||
3.4 Detection of severe acute respiratory syndrome-coronavirus-2 (SARS-CoV-2)
Recently, graphene biosensors were applied in the development of point-of-care (POC) testing (POCT) devices for the detection of coronavirus disease-19 (COVID-19), an ongoing pandemic the world is suffering from. The rapid and sensitive detection of SARS-CoV-2, the causative pathogen of COVID-19, is an ongoing global challenge that is associated with large-scale diagnosis in order to downregulate its spread within the communities. It demands early identification of infection in presymptomatic and asymptomatic individuals [162,163]. There remains an urgent need for a rapid and precise diagnostic method for the detection and screening of the disease. The graphene-based biosensors have attracted much attention in the outbreak owing to their extraordinary properties  and have emerged as a successful application tool to detect COVID-19. Antibody-conjugated graphene sheets could rapidly detect target viral proteins and were used for large-scale screening and development of biosensors . The available conventional technology such as RT-PCR is time-consuming, labor-intensive, and scarcely available in remote areas. These POC biosensors are typically low-cost, user-friendly, and have remarkable potential as medical diagnostics . These biosensors are now a future diagnostic approach for COVID-19 as clinical diagnostics  owing to their accuracy, affordability, and portability . The introduction of nanomaterials unquestionably enhanced the performance of graphene biosensors, and the sensing abilities of these biosensors are of a peerless level of ultrasensitivity . Table 5 summarizes the graphene-based biosensors developed so far in the point-of-care testing (POCT) for COVID-19.
|Type of graphene biosensor||Technology/nanotechnology used||Time of detection||Limit of detection (LOD)||Outcomes of the study||Reference|
|Quantitative paper-based electrochemical sensor chip||AuNPs capped with highly specific antisense oligonucleotides (ssDNA) aimed to target nucleocapsid phosphoprotein (N-gene)||Less than 5 min||Significant amplification in the output signal in the presence of SARS-CoV-2-RNA; Sensitivity: 231 (copies μL–1)−1; LOD: 6.9 copies μL−1||The developed sensor showed almost 100% accuracy, specificity, and sensitivity|||
|Multiplexed, portable, wireless electrochemical biosensor||Laser engraved graphene electrodes||—||—||The developed sensor could detect viral antigen N-protein, as well as IgM and IgG antibodies along with the C-reactive protein (CRP), the inflammatory biomarker|||
|FET-based biosensor||Graphene sheets of the FET were coated with specific SARS-CoV-2 monoclonal antibodies against S-protein||—||FET device could detect SARS-CoV-2; LOD (in the culture medium): 1.6 × 101 Pfu mL−1; LOD (in clinical samples): 2.42 × 102 copies mL−1||Successful fabrication of the FET biosensor as a highly sensitive immunological diagnostic method|||
|A novel biosensor based on bioelectric recognition assay||Human chimeric spike S1 antibody immobilized on membrane-engineered mammalian cells||Ultra-rapid manner (3 min)||1 fg mL−1||Configured biosensor could be applied as a ready-to-use tool in the mass screening of SARS-CoV-2 antigens. No sample processing step is required|||
|CRISPR-based assay||Based on CRISPR complex (Cas12a/gRNA) attached to a fluorescent probe that could detect targeted amplicons produced by RT-PCR||∼50 min||LOD of 2 copies per sample||Results demonstrated rapid analytical sensitivity and robust diagnostic performance to improve the current COVID-19 screening.|||
|Simple immunosensor integrated onto a microfluidic chip||Utilizes the dual-labeled magnetic nanobeads immunomagnetic enrichment and signal amplification||Rapid quantification (<1 h) of SARS-CoV-2 antigen in whole serum samples||Rapid detection of SARS-CoV-2 protein biomarkers; highly sensitive; less than 50 µL serum sample required.||Functionality validated by detecting SARS-CoV-2 N-protein; a promising platform for POCT|||
|Ultrasensitive electrochemical detection using calixarene functionalized GO||Based on super sandwich type recognition strategy; practical detection of SARS-CoV-2 RNA using electrochemical Smartphone without amplification of nucleic acids and reverse transcription||—||LOD of the clinical specimen was 200 copies mL−1||Both in silico analysis and actual testing showed high selectivity and high specificity|||
|Electrochemical immunosensor||Usage of magnetic beads as immunological chain support with secondary antibodies coupled with alkaline phosphatase used as an immunological label; applied for the detection of both S- and N-protein of SARS-CoV-2||30 min||The analytical features of the electrochemical immunoassay were assessed using N- and S-protein standard solutions with untreated saliva; detection limit: 19 and 8 ng mL−1, respectively, for S- and N-proteins||An analytical tool with high potentiality for market entry for SARS-CoV-2 detection in untreated saliva|||
|Voltammetric genosensor||Hexathia-18-crown-6 (HT18C6) modified with Ag + ions used as redox probe; carbon paste electrode (CPE) coated with HT18C6-Ag and modified further using chitosan and PAMAM dendrimer-coated silicon quantum dots (SiQDs-PAMAM)||—||Concentration range: 1.0 pM to 8.0 nM; LOD: 0.3 pM. Against SARS-CoV-2 RdRP||Detection of SARS-CoV-2 in human sputum|||
|Label-free paper-based electrochemical biosensor||Immunosensor designed for the detection of immunoglobulin against SARS-CoV-2 with high specificity and sensitivity||—||—||Opens new possibilities for diagnosing COVID-19|||
|FET||Portable bifunctional electrical detector based on graphene FET for the detection of SARS-CoV-2 via nucleic acid hybridization or Ag–Ab interaction||Exhibited rapid detection speed (∼10 min for nucleic acid detection and ∼5 min for immunoassay)||—||Efficient and accurate tool for high-throughput point of care testing of COVID-19|||
The breakthrough in the discovery of graphene-based biosensors for the diagnosis of COVID-19 was made when a graphene-based electrochemical biosensor coupled with an electrical readout setup was developed, which was selectively able to detect the SARS-CoV-2 genetic material . The biosensor was made selective by integrating thiol-modified antisense oligonucleotides (ssDNA), which were specific for the N-gene (nucleocapsid phosphoprotein) of SARS-CoV-2. The sensitivity of the detector was further enhanced when the thiol-modified ssDNA-capped gold nanoparticles (AuNPs) were applied on the gold electrode. Similarly, a wireless graphene-based telemedicine platform known as the SARS-CoV-2 RapidPlex was developed, which could successfully detect the nucleocapsid protein (NP) as well as specific immunoglobulins against the spike protein (S1) (S1-IgG and S1-IgM), in both blood and saliva of the patients . The detector consisted of laser-engraved graphene sensor arrays that were proved to be a highly convenient, rapid, accurate, and stage-specific tool for the detection of the virus. 1-Pyrene butyric acid (PBA) was utilized as the linker to attach the receptors onto the graphene surface.
In another study, the SARS-CoV-2 spike protein antibody was immobilized onto the fabricated graphene-based device using 1-pyrene butyric acid N-hydroxysuccinimide ester (PBASE) as an interface coupling agent . The developed biosensor showed an excellent LOD of 1 fg mL−1 of the viral spike protein. The sensitivity of the biosensor was assessed using a control experiment that showed that the spike protein was essential for specific binding with the viral antigen. The selectivity was confirmed when the developed COVID-19 FET did not exhibit any response to MERS-CoV spike proteins. Recently, another graphene-based FET device was developed as a portable bifunctional electrical detector through either nucleic acid hybridization or antigen–antibody protein interaction . The developed biosensor showed ultra-low detection limits in the range of 0.1–1 fg mL−1 and was able to detect the pathogen in real samples. The biosensor was fabricated using PBASE in acetonitrile and was exposed to ssDNA probe or antigen protein.
4 Patents and clinical trials on graphene-based biosensors
A number of patents were granted worldwide on graphene-based biosensor devices and the methods of manufacturing. The first patent was granted in the year 2010, a few years after the discovery of graphene in which the configuration of graphene device was described . The patented device consisted of two electrodes, three layered structures (conductive, insulating, and graphene), and a superconducting dopant island. The graphene layer was adsorbed to the electrodes. In between the electrodes, the dopant island was coupled to an exposed surface of the graphene layer. This device was applied in the chemical detection by applying a voltage to the conductive layer and observing the voltage response of the dopant island. Subsequently, in 2011, a worldwide patent was granted on the graphene-based biosensor in which the method of preparation of the graphene biosensor was described that helped to detect biological molecules . This sensor consisted of the graphene structure (thickness of about 10 atomic layers of graphene), two electric contacts or micro electrodes (that determine the conductivity), and at least one linker (one of the linkers has a biological molecule binding affinity). The patterned graphene structure was composed of at least one (three-dimensional) channel of about 100 μm and two microelectrodes were arranged on opposite sides of the channel. The linker could be an aniline group, amino group, or a diazonium salt that could be changed according to the biological sample to be tested. The change in conductivity in the prepared sensor measured the biological molecule.
This led to an increase in the number of patents in the following years on graphene-based biosensors owing to a much expected attraction of scientists worldwide. In 2013, a US patent was granted in which the graphene biosensor was prepared using graphene-coated electrodes that were linked to one to six layers of the flexible substrate through the enzyme lactate oxidase (biosensing element) . Graphene electrodes consisted of two terminals: negative (second end) and positive (first end) terminals. Once the analyte in the sample is in contact with the graphene electrode, the voltage might be applied and the concentration was measured via the electric current response. In the same year, another graphene-based biosensor device received the patented status where the graphene nanosheet modified with chitosan were coated on glassy carbon electrodes and were used as sensing agents for polynucleotide and mutation detection using voltammetry . Another breakthrough in the research on graphene-based biosensors came when a patent on FET was developed for the detection of biomolecular samples . This sensor consisted of a graphene layer (semiconductor material) bound with ligand-binding protein that helped to detect protein-based substances.
Another graphene-based FET biosensor device was developed by modifying their edges with functional groups that helped in detecting the sample using an analyzer by measuring the change in the current generated by the sample connected to the functional group. Thin-film graphitic layers made up of many graphene layers were added to a base in the desired pattern and altered for better electrode connection . A novel strategy for the detection of samples present in food was developed using electrochemical DNA graphene or biochip biosensor. Their detection was based on the mechanism of DNA (present in the sample)–redox (ruthenium hexamine molecule) electrostatic complex, and their subsequent nonspecific adsorption on the graphene surface. The developed biosensor was able to detect meat samples using isothermal amplification of DNA and electrochemical detection via square wave voltammetry . Two Chinese patents were granted recently in the years 2018 and 2019 using graphene-based biosensors for the detection of guanine ribose  and cancer marker microRNA  using 3D graphene biosensors. These biosensors consisted of a graphene layer over a glass substrate where indium tin oxide was arranged on the sides of the sensor. This 3D biosensor showed a number of advantages including ease of operation and use, improved specificity at lower operating voltages, and even great safety. Very recently, a graphene biosensor was designed and manufactured using GNP ink, which was deposited on the surface of the substrate to provide at least one sensing layer. This layer was processed via photonic curing to generate a graphene electrode vertically arranged graphene sheets and used for plasma treatment for functionalization, which was used for the identification of biological molecules .
Various nongraphene biosensors are being tested in clinical trials for the identification of various diseases, but graphene-based biosensors are only a few. A new approach based on the photoelectrochemical immunosensor employed graphene quantum dots in conjunction with Si nanowires for the early detection of myocardial infarction was under clinical trial but is not yet recruiting . They aimed to examine 100 people above the age of 18 who complained of chest pain to see if they had an acute myocardial infarction.
5 Biomedical graphene biosensors – market trends, opportunities, and future perspectives
Graphene often heralded as the wonder material is an advanced 2D carbon-based material of the 21st century having exceptional properties of light-weightedness, high strength, super flexibility, excellent superconductivity, and having a paramount potential in improving the human life quality. Today, biosensors have made a huge impact in various biosensing platforms as electrochemical biosensors, fluorescent biosensors, and graphene biosensors for enzymatic biosensing and immunosensing applications. The superconductive material graphene is a low-cost ideal material for the construction of sensors and biosensors-based devices for biomedical applications . Graphene is considered one of the most advanced materials in human healthcare as biosensing and diagnostic tool and this has accelerated medical diagnosing to new dimensions. It has successfully revolutionized our understanding of the treatment of deadly diseases through its derivatives and hybrids-based biosensors and their march toward the marketplace is at a high pace and more of these are expected to come into the market in the next decade as high-end diagnostic tools in POCT .
As research and development are growing each year, biosensors are becoming a commercial reality. But, before becoming a commercially significant device, the graphene-based biosensors are bound to face initial and primary challenges such as quality control, scalability, and durability issues that should be resolved transparently. The intrinsic properties of graphene, their integration with other functional materials, fabrication of devices, and processing steps need close considerations . The market forecast reports on biosensors were shared for understanding more about their market trends and opportunities. The Biomedical Sensor Market - Forecast Report (2021–2026) stated that these biosensors adjusted themselves according to the genetic make-up of each patient and are programmed to send alarm signals when anomalies or unexpected body readings are registered in real-time . Biomedical sensor devices greatly improved early detection of health problems by measuring blood pressure remotely, detection of toxins in blood, analysis of glucose, lactate, and glutamine in aqueous media, and analysis of other complex biological media.
Similarly, the Frost and Sullivan Analysis Report (2018–2023) on biosensor market forecast expected growth in the biosensor market at a 12% compound annual growth rate during 2018–2023 from $17.7 billion in 2018 to reach up to $31.2 billion by the end of 2023 . The key application areas and segments marked by them included point-of-care home diagnostics in the healthcare system, food, water, and air quality monitoring, agriculture and security, etc. Wearable biosensors for the noninvasive monitoring of heart rate, breathing rate, glucose, disease diagnostics, and detection are also mentioned in their report. The US National Institute of Health would encourage and fund biosensor-related research activities. The nano-biosensors have promising applications in the biomedical sector and diagnostics because of their improved specificity and selectivity. Other than the upward market trend of nano-biosensors and wearable biosensors, the digestible biosensors, silicon photonic biosensors, implantable biosensors, and touch-based in-vehicle sensors are also having promising future in this area of biosensing .
The Graphene Market and 2D Materials Assessment Report (2021–2031) forecasted for 18 key applications areas and the movement of graphene biosensors from the laboratory to the commercial market in the coming decades. According to this assessment report, the forecast was made that the graphene market will continue to grow from <$100 m in 2020 up to $700 m by 2031. This success will not be immediate or overnight and will be because of continued efforts by global research and commercialization efforts. In this regard, nanoplatelets are closest to commercial success, and progress toward their standardization, safety, legislation, quantification is progressive and quite evident . Very recently, a Graphene Research Hub was launched in 2017 as a collaborative platform in academia and industry at the University of Adelaide with the aim of enabling the development of a sustainable graphene-based industry in Australia .
There is a race to the commercialization of graphene-based biosensors and bringing them to market will change the way diseases are diagnosed and treatment is delivered. Patients will receive the test results fast, the diagnosis will be at the site in minutes, and treatment could begin immediately thus saving valuable and precious time . For instance, very recently, researchers from the University of Illinois, Grainger College of Engineering, developed rapid, ultrasensitive testing using a paper-based graphene electro-chemical biosensor that can detect the COVID-19 virus in less than 5 min .
The understanding of physics and nanotechnology goes hand-in-hand and it holds potential in improving the quality, cost of biological testing, speed, and capability to analyze the resulting complex data. Biosensors enable biotechnicians to control the precise biological data . Based on their pharmaceutical applications, the biomedical biosensors’ market has been segmented as cardiac care, pain management, drug discovery, diagnostics, and genomics. The global market trends and opportunities show that wearable biosensors are in an upward trend, especially in diabetics and cardiovascular diseases [199–201].
6 Conclusions and future perspectives
A vast variety of graphene-based nanomaterials consisting of pristine graphene, GO, rGO, and graphene quantum dots are used for the preparation of graphene-based biosensors. These biosensors showed a plethora of applications in biomedical and nonbiomedical fields for the detection of target molecules. The uncountable unique properties of graphene including mobility, large surface area, transparency, nontoxicity, tensile strength, and superior electrical and thermal conductivity allowed the functionalization and immobilization steps leading to the development of sensitive and accurate biosensors. Graphene-based materials can be employed and integrated into designing biosensing platforms resulting in the development of ultrasensitive biosensors, which can be utilized for the early detection of many infectious and noninfectious diseases. As the research on graphene-based nanomaterials is growing, the excellent and unmatched potential of these materials is being revealed for specific purposes. The added advantages of graphene-based biosensors include cost-effectiveness, miniaturization, accuracy, and reproducibility, which showed promising market potential and large-scale commercialization of these biosensors as an alternative to conventional sensing techniques. However, there are several drawbacks associated with graphene-based technology that cannot be ignored. For instance, graphene, owing to its ability to adsorb nontarget molecules may result in giving false-positive detection, especially if noncovalent functionalization methods are used. On the other hand, covalent functionalization methods are complex, and precise conditional control is required to achieve it. Moreover, the loading of biomolecules onto the graphene surface is affected by external environmental factors such as temperature, pH, salt concentration, as well as the intrinsic properties of graphene such as type, molecular weight, surface properties, etc. Indeed, more studies are warranted on graphene and its functionalized derivatives with lesser impurities and improved methods of manufacturing, which would contribute to the growing momentum toward designing new biosensing devices suitable for POCT and improve the quality of the healthcare system worldwide.
The authors extend their appreciation to the deputyship for Research & Innovation, Ministry of Education in Saudi Arabia for funding this research work through the project with no. ISP20 – 3.
Funding information: This work was funded by the Deanship of Scientific Research, Jazan University, Jazan, Saudi Arabia, under the Jazan University Research Groups Funding Program for the Ministry of Education’s initiative for institutional funding (Project no. ISP20 – 3).
Author contributions: HAA and WA developed the concept of the manuscript, WA, BM, MZH, MA, and SJ conducted the literature survey; WA, BM, MZH, and SJ developed the methodology and performed data curation. WA, HAA, BM, SJ, MZH, and MA wrote the draft manuscript, while MAB, AN, and HAA performed the writing-review and editing. HAA, MAB, and AN supervised the work. All authors have accepted responsibility for the entire content of this manuscript and approved its submission.
Conflict of interest: The authors state no conflict of interest.
Data availability statement: The datasets generated during and/or analysed during the current study are available from the corresponding author on reasonable request.
 Haque R, Kress K, Wood S, Jackson TF, Lyerly D, Wilkins T, et al. Diagnosis of pathogenic entamoeba histolytica infection using a stool elisa based on monoclonal antibodies to the galactose-specific adhesin. J Infect Dis. 2018;167:247–9.10.1093/infdis/167.1.247Search in Google Scholar
 Josephson KL, Gerba CP, Pepper IL. Polymerase chain reaction detection of nonviable bacterial pathogens. Appl Env Microbiol. 1993;59:3513–5.10.1128/aem.59.10.3513-3515.1993Search in Google Scholar
 Wilson WJ, Strout CL, DeSantis TZ, Stilwell JL, Carrano AV, Andersen GL. Sequence-specific identification of 18 pathogenic microorganisms using microarray technology. Mol Cell Probes. 2002;16:119–27.10.1006/mcpr.2001.0397Search in Google Scholar
 Lindsley MD, Mekha N, Baggett HC, Surinthong Y, Autthateinchai R, Sawatwong P, et al. Evaluation of a newly developed lateral flow immunoassay for the diagnosis of cryptococcosis. Clin Infect Dis. 2011;53:321–5.10.1093/cid/cir379Search in Google Scholar
 Zhu Y, Murali S, Cai W, Li X, Suk JW, Potts JR, et al. Graphene and graphene oxide: synthesis, properties, and applications. Adv Mater. 2010;22:3906–24.10.1002/adma.201001068Search in Google Scholar PubMed
 Janegitz BC, Silva TA, Wong A, Ribovski L, Vicentini FC, Taboada Sotomayor MDP, et al. The application of graphene for in vitro and in vivo electrochemical biosensing. Biosens Bioelectron. 2017;89:224–33.10.1016/j.bios.2016.03.026Search in Google Scholar PubMed
 Wang Y, Li Z, Wang J, Li J, Lin Y. Graphene and graphene oxide: biofunctionalization and applications in biotechnology. Trends Biotechnol. 2011;29:205–12.10.1016/j.tibtech.2011.01.008Search in Google Scholar PubMed PubMed Central
 Liu J, Tang J, Gooding JJ. Strategies for chemical modification of graphene and applications of chemically modified graphene. J Mater Chem. 2012;22:12435.10.1039/c2jm31218bSearch in Google Scholar
 Shams N, Lim HN, Hajian R, Yusof NA, Abdullah J, Sulaiman Y, et al. Electrochemical sensor based on gold nanoparticles/ethylenediamine-reduced graphene oxide for trace determination of fenitrothion in water. RSC Adv. 2016;6(92):89430–9.10.1039/C6RA13384CSearch in Google Scholar
 Geim AK, Novoselov KS. The rise of graphene, nanoscience and technology: a collection of reviews from nature journals. World Scientific; 2010. p. 11–9.10.1142/9789814287005_0002Search in Google Scholar
 Park HJ, Meyer J, Roth S, Skákalová V. Growth and properties of few-layer graphene prepared by chemical vapor deposition. Carbon. 2010;48(4):1088–94.10.1016/j.carbon.2009.11.030Search in Google Scholar
 Krajewska A, Pasternak I, Sobon G, Sotor J, Przewloka A, Ciuk T, et al. Fabrication and applications of multi-layer graphene stack on transparent polymer. Appl Phys Lett. 2017;110(4):041901.10.1063/1.4974457Search in Google Scholar
 Nieto A, Lahiri D, Agarwal A. Synthesis and properties of bulk graphene nanoplatelets consolidated by spark plasma sintering. Carbon. 2012;50(11):4068–77.10.1016/j.carbon.2012.04.054Search in Google Scholar
 Alam SN, Sharma N, Kumar L. Synthesis of graphene oxide (GO) by modified hummers method and its thermal reduction to obtain reduced graphene oxide (rGO). Graphene. 2017;6(1):1.10.4236/graphene.2017.61001Search in Google Scholar
 Compton OC, Nguyen ST. Graphene oxide, highly reduced graphene oxide, and graphene: versatile building blocks for carbon-based materials. Small. 2010;6(6):711–23.10.1002/smll.200901934Search in Google Scholar PubMed
 Eda G, Chhowalla M. Chemically derived graphene oxide: towards large-area thin-film electronics and optoelectronics. Adv Mater. 2010;22(22):2392–415.10.1002/adma.200903689Search in Google Scholar PubMed
 Kang X, Wang J, Wu H, Liu J, Aksay I, Lin Y. A graphene-based electrochemical sensor for sensitive detection of paracetamol. Talanta. 2010;81:754–9.10.1016/j.talanta.2010.01.009Search in Google Scholar PubMed
 Du M, Yang T, Ma S, Zhao C, Kui J. Ionic liquid-functionalized graphene as modifier for electrochemical and electrocatalytic improvement: comparison of different carbon electrodes. Anal Chim Acta. 2011;690:169–74.10.1016/j.aca.2011.01.051Search in Google Scholar PubMed
 Chen L, Tang Y, Wang Ke, Liu C, Luo S. Direct electrodeposition of reduced graphene oxide on glassy carbon electrode and its electrochemical application. Electrochem Comm. 2011;13:133–7.10.1016/j.elecom.2010.11.033Search in Google Scholar
 Gan X, Zhao H. A review: nanomaterials applied in graphene-based electrochemical biosensors. Sens Mater. 2015;27:191–215.Search in Google Scholar
 Krishnan SK, Singh E, Singh P, Meyyappan M, Nalwa HS. A review on graphene-based nanocomposites for electrochemical and fluorescent biosensors. RSC Adv. 2019;9:8778–81.10.1039/C8RA09577ASearch in Google Scholar
 Azizi-Lalabadi M, Jafari SM. Bio-nanocomposites of graphene with biopolymers; fabrication, properties, and applications. Adv Colloid Interface Sci. 2021;292:102416.10.1016/j.cis.2021.102416Search in Google Scholar PubMed
 Antonatos N, Ghodrati H, Sofer Z. Elements beyond graphene: current state and perspectives of elemental monolayer deposition by bottom-up approach. Appl Mater Today. 2020;18:100502.10.1016/j.apmt.2019.100502Search in Google Scholar
 Ikram R, Jan BM, Ahmad W. An overview of industrial scalable production of graphene oxide and analytical approaches for synthesis and characterization. J Mater Res Technol. 2020;9:11587–610.10.1016/j.jmrt.2020.08.050Search in Google Scholar
 Cho IH, Kim DH, Park S. Electrochemical biosensors: perspective on functional nanomaterials for on-site analysis. Biomater Res. 2020;24:1–12.10.1186/s40824-019-0181-ySearch in Google Scholar PubMed PubMed Central
 Prattis I, Hui E, Gubeljak P, Kaminski GS, Schierle A, Lombardo LG, et al. Graphene for biosensing applications in point-of-care testing. Trends Biotechnol. 2021;39:1–13.10.1016/j.tibtech.2021.01.005Search in Google Scholar PubMed
 Ahmad R, Wolfbeis OS, Hahn YB, Alshareef HN, Torsi L, Salama KN. Deposition of nanomaterials: a crucial step in biosensor fabrication. Mater Today Commun. 2018;17:289–321.10.1016/j.mtcomm.2018.09.024Search in Google Scholar
 Chong WS, Gan SX, Al-Tuwirit HM, Chong WY, Lim CS, Ahmad H. Nanolitre solution drop-casting for selective area graphene oxide coating on planar surfaces. Mater Chem Phys. 2020;249:122970.10.1016/j.matchemphys.2020.122970Search in Google Scholar
 Kamil MP, Kim MJ, Ko YG. Direct electro-co-deposition of Ni-reduced graphene oxide composite coating for anti-corrosion application. Mater Lett. 2020;273:1–4.10.1016/j.matlet.2020.127911Search in Google Scholar
 Barkauskas J, Mikoliunaite L, Paklonskaite I, Genys P, Petroniene JJ, Morkvenaite-Vilkonciene I, et al. Single-walled carbon nanotube based coating modified with reduced graphene oxide for the design of amperometric biosensors. Mater Sci Eng C. 2019;98:515–23.10.1016/j.msec.2019.01.005Search in Google Scholar PubMed
 Kumar S, Gupta N, Malhotra BD. Ultrasensitive biosensing platform based on yttria doped zirconia-reduced graphene oxide nanocomposite for detection of salivary oral cancer biomarker. Bioelectrochemistry. 2021;140:107799.10.1016/j.bioelechem.2021.107799Search in Google Scholar PubMed
 El barghouti M, Akjouj A, Mir A. Design of silver nanoparticles with graphene coatings layers used for LSPR biosensor applications. Vacuum. 2020;180:109497.10.1016/j.vacuum.2020.109497Search in Google Scholar
 Yousaf HMZ, Kim SW, Hassan G, Karimov K, Choi KH, Sajid M. Highly sensitive wide range linear integrated temperature compensated humidity sensors fabricated using electrohydrodynamic printing and electrospray deposition. Sens Actuators B Chem. 2020;308:127680.10.1016/j.snb.2020.127680Search in Google Scholar
 Mishra RK, Nawaz MH, Hayat A, Nawaz MAH, Sharma V, Marty JL. Electrospinning of graphene-oxide onto screen printed electrodes for heavy metal biosensor. Sens Actuators B Chem. 2017;247:366–73.10.1016/j.snb.2017.03.059Search in Google Scholar
 Pavinatto A, Mercante LA, Facure MHM, Pena RB, Sanfelice RC, Mattoso LHC, et al. Ultrasensitive biosensor based on polyvinylpyrrolidone/chitosan/reduced graphene oxide electrospun nanofibers for 17α – Ethinylestradiol electrochemical detection. Appl Surf Sci. 2018;458:431–7.10.1016/j.apsusc.2018.07.035Search in Google Scholar
 Lahcen AA, Rauf S, Beduk T, Durmus C, Aljedaibi A, Timur S, et al. Electrochemical sensors and biosensors using laser-derived graphene: a comprehensive review. Biosens Bioelectron. 2020;168:112565.10.1016/j.bios.2020.112565Search in Google Scholar PubMed
 López Marzo AM, Mayorga-Martinez CC, Pumera M. 3D-printed graphene direct electron transfer enzyme biosensors. Biosens Bioelectron. 2020;151:111980.10.1016/j.bios.2019.111980Search in Google Scholar PubMed
 Wajahat M, Kim JH, Ahn J, Lee S, Bae J, Pyo J, et al. 3D printing of Fe3O4 functionalized graphene-polymer (FGP) composite microarchitectures. Carbon N Y. 2020;167:278–84.10.1016/j.carbon.2020.05.045Search in Google Scholar
 Yoon H, Nah J, Kim H, Ko S, Sharifuzzaman M, Barman SC, et al. A chemically modified laser-induced porous graphene based flexible and ultrasensitive electrochemical biosensor for sweat glucose detection. Sens Actuators B Chem. 2020;311:127866.10.1016/j.snb.2020.127866Search in Google Scholar
 Perumal V, Mohamed NM, Saheed MSM, Saheed MSM. Novel hydrothermal growth of ZnO/NiO hybrids nanostructures on 3D graphene. Mater Today Proc. 2019;16:2408–13.10.1016/j.matpr.2019.06.146Search in Google Scholar
 Low SS, Tan MTT, Loh HS, Khiew PS, Chiu WS. Facile hydrothermal growth graphene/ZnO nanocomposite for development of enhanced biosensor. Anal Chim Acta. 2016;903:131–41.10.1016/j.aca.2015.11.006Search in Google Scholar PubMed
 Liu M, Duan Y, Wang Y, Zhao Y. Diazonium functionalization of graphene nanosheets and impact response of aniline modified graphene/bismaleimide nanocomposites. Mater Des. 2014;53:466–74.10.1016/j.matdes.2013.07.027Search in Google Scholar
 Craciun MF, Khrapach I, Barnes MD, Russo S. Properties and applications of chemically functionalized graphene. J Phys Condens Matter. 2013;25(42):423201.10.1088/0953-8984/25/42/423201Search in Google Scholar PubMed
 Daukiya L, Seibel J, De, Feyter S. Chemical modification of 2D materials using molecules and assemblies of molecules. Adv Phys. 2019;4(1):1625723.10.1080/23746149.2019.1625723Search in Google Scholar
 Liu L, Ward RM, Schomaker JM. Mechanistic aspects and synthetic applications of radical additions to allenes. Chem Rev. 2019;119(24):12422–90.10.1021/acs.chemrev.9b00312Search in Google Scholar PubMed PubMed Central
 Yu DS, Kuila T, Kim NH, Lee JH. Enhanced properties of aryl diazonium salt-functionalized graphene/poly(vinyl alcohol) composites. Chem Eng J. 2014;245:311–22.10.1016/j.cej.2014.02.025Search in Google Scholar
 Ma X, Li F, Wang Y, Hu A. Functionalization of pristine graphene with conjugated polymers through diradical addition and propagation. Chem Asian J. 2012;7(11):2547–50.10.1002/asia.201200520Search in Google Scholar PubMed
 Mahouche-Chergui S, Gam-Derouich S, Mangeney C, Chehimi MM. Aryl diazonium salts: a new class of coupling agents for bonding polymers, biomacromolecules and nanoparticles to surfaces. Chem Soc Rev. 2011;40(7):4143–66.10.1039/c0cs00179aSearch in Google Scholar PubMed
 Komeily-Nia Z, Chen JY, Nasri-Nasrabadi B, Lei WW, Yuan B, Zhang J, et al. The key structural features governing the free radicals and catalytic activity of graphite/graphene oxide. Phys Chem Chem Phys. 2020;22(5):3112–21.10.1039/C9CP05488JSearch in Google Scholar PubMed
 Maschio G, Lister DG, Casson Moreno V. Use of screening analysis calorimetry in the study of peroxides decomposition. Chem Eng Trans. 2010;19:347–52.Search in Google Scholar
 Sanchez, J, Myers, TN. Organic peroxides. Kirk-Othmer encyclopedia of chemical technology. Vol. 18. 5th edn. Hoboken, NJ: John Wiley & Sons; 2006. p. 489–96.Search in Google Scholar
 Aiguo H. Bergman cyclization polymerization. Acta Polym Sin. 2016;12:1635–44.Search in Google Scholar
 Raji M, Zari N, Qaiss AK, Bouhfid R. Chapter 1 – Chemical preparation and functionalization techniques of graphene and graphene oxide. Micro and nano technologies, functionalized graphene nanocomposites and their derivatives. New York, NY: Elsevier; 2019. p. 1–20.10.1016/B978-0-12-814548-7.00001-5Search in Google Scholar
 Li P-P, Chen Y, Zhu J, Feng M, Zhuang X, Lin Y, et al. Charm-bracelet-type poly(N-vinylcarbazole) functionalized with reduced graphene oxide for broadband optical limiting. Chem – Eur J. 2011;17(3):780–5.10.1002/chem.201002431Search in Google Scholar PubMed
 Xu X, Chen J, Luo X, Lu J, Zhou H, Wu W, et al. Poly(9,9′-diheylfluorene carbazole) functionalized with reduced graphene oxide: convenient synthesis using nitrogen-based nucleophiles and potential applications in optical limiting. Chem – Eur J. 2012;18(45):14384–91.10.1002/chem.201201360Search in Google Scholar PubMed
 Parthasarathy K, Cheng C-H. Metal-Mediated and metal-catalyzed [2 + 2] cycloadditions. In: Knochel P, editor. Comprehensive organic synthesis II (2nd edn.). New York, NY: Elsevier; 2014. p. 222–72.10.1016/B978-0-08-097742-3.00507-3Search in Google Scholar
 Ferrándiz-Saperas M, Ghisolfi A, Cazorla-Amorós D, Nájera C, Sansano JM. Multilayer graphene functionalized through thermal 1,3-dipolar cycloadditions with imino esters: a versatile platform for supported ligands in catalysis. Chem Commun (Camb). 2019;55(52):7462–5.10.1039/C9CC00939FSearch in Google Scholar PubMed
 Yu M, Chen C, Liu Q, Mattioli C, Sang H, Shi G, et al. Long-range ordered and atomic-scale control of graphene hybridization by photocycloaddition. Nat Chem. 2020;12(11):1035–41.10.1038/s41557-020-0540-2Search in Google Scholar PubMed
 Tan KH, Sattari S, Beyranvand S, Faghani A, Ludwig K, Schwibbert K, et al. Thermoresponsive amphiphilic functionalization of thermally reduced graphene oxide to study graphene/bacteria hydrophobic interactions. Langmuir. 2019;35(13):4736–46.10.1021/acs.langmuir.8b03660Search in Google Scholar PubMed
 Oh C-R, Lee S-H, Park J-H, Lee D-S. Thermally self-healing graphene-nanoplate/polyurethane nanocomposites via Diels–Alder reaction through a one-shot process. Nanomaterials (Basel). 2019;9(3):434.10.3390/nano9030434Search in Google Scholar PubMed PubMed Central
 Zhang J, Hu K, Ouyang Q, Gui Q, Chen X. One-step functionalization of graphene via Diels–Alder reaction for improvement of dispersibility. Front Mater Sci. 2020;14:198–210.10.1007/s11706-020-0501-0Search in Google Scholar
 Li J, Li M, Zhou LL, Lang SY, Lu HY, Wang D, et al. Click and patterned functionalization of graphene by Diels–Alder reaction. J Am Chem Soc. 2016;138(24):7448–51.10.1021/jacs.6b02209Search in Google Scholar PubMed
 Stuyver T, Danovich D, De Proft F, Shaik S. Electrophilic aromatic substitution reactions: mechanistic landscape, electrostatic and electric-field control of reaction rates, and mechanistic crossovers. J Am Chem Soc. 2019;141(24):9719–30.10.1021/jacs.9b04982Search in Google Scholar PubMed
 Shellard PM, Srisubin T, Hartmann M, Butcher J, Fei F, Cox H, et al. A versatile route to edge-specific modifications to pristine graphene by electrophilic aromatic substitution. J Mater Sci. 2020;55(24):10284–302.10.1007/s10853-020-04662-ySearch in Google Scholar PubMed PubMed Central
 Khan R, Nakagawa R, Campeon B, Nishina Y. A simple and robust functionalization of graphene for advanced energy devices. ACS Appl Mater Interfaces. 2020;12(11):12736–42.10.1021/acsami.9b21082Search in Google Scholar PubMed
 Guan F, Ren H, Yu L, Cui Q, Zhao W, Liu J. Nitrated graphene oxide derived from graphite oxide: a promising energetic two-dimensional material. Nanomaterials (Basel). 2020;11(1):58.10.3390/nano11010058Search in Google Scholar PubMed PubMed Central
 Wu JM, Jing GJ, Lu XL, Lei TY, Wang SX, Cheng X, et al. The effect of sulfonated graphene on the rheological properties of cement paste. J Nanosci Nanotechnol. 2020;20(12):7495–505.10.1166/jnn.2020.18871Search in Google Scholar PubMed
 Hu F, Patel M, Luo F, Flach C, Mendelsohn R, Garfunkel E, et al. Graphene-catalyzed direct Friedel-Crafts alkylation reactions: mechanism, selectivity, and synthetic utility. J Am Chem Soc. 2015;137(45):14473–80.10.1021/jacs.5b09636Search in Google Scholar PubMed
 Wang A, Ye J, Humphrey MG, Zhang C. Graphene and carbon-nanotube nanohybrids covalently functionalized by porphyrins and phthalocyanines for optoelectronic properties. Adv Mater. 2018;30(17):e1705704.10.1002/adma.201705704Search in Google Scholar PubMed
 Openda YI, Sen P, Managa M, Nyokong T. Acetophenone substituted phthalocyanines and their graphene quantum dots conjugates as photosensitizers for photodynamic antimicrobial chemotherapy against Staphylococcus aureus. Photodiag Photodyn Ther. 2020;29:101607.10.1016/j.pdpdt.2019.101607Search in Google Scholar PubMed
 Cardano F, Frasconi M, Giordani S. Photo-responsive graphene and carbon nanotubes to control and tackle biological systems. Front Chem. 2018;6:102.10.3389/fchem.2018.00102Search in Google Scholar PubMed PubMed Central
 Xu Y, Liu Z, Zhang X, Wang Y, Tian J, Huang Y, et al. A graphene hybrid material covalently functionalized with porphyrin: synthesis and optical limiting property. Adv Mater. 2009;21:1275.10.1002/adma.200801617Search in Google Scholar
 Zhou Y, Fang Y, Ramasamy RP. Non-covalent functionalization of carbon nanotubes for electrochemical biosensor development. Sens (Basel). 2019;19(2):392.10.3390/s19020392Search in Google Scholar PubMed PubMed Central
 Kim KS, Suh SB, Kim JC, Hong BH, Lee EC, Yun S, et al. Assembling phenomena of calixhydroquinone nanotube bundles by one-dimensional short hydrogen bonding and displaced pi-pi stacking. J Am Chem Soc. 2002;124:14268–79.10.1021/ja0259786Search in Google Scholar PubMed
 Xu Y, Bai H, Lu G, Li C, Shi G. Flexible graphene films via the filtration of water-soluble noncovalent functionalized graphene sheets. J Am Chem Soc. 2008;130(18):5856–7.10.1021/ja800745ySearch in Google Scholar PubMed
 Zhang C, Ren J, Zhou J, Cui M, Li N, Han B, et al. Facile fabrication of a 3,4,9,10-perylene tetracarboxylic acid functionalized graphene-multiwalled carbon nanotube-gold nanoparticle nanocomposite for highly sensitive and selective electrochemical detection of dopamine. Analyst. 2018;143(13):3075–84.10.1039/C8AN00559ASearch in Google Scholar
 Monteiro AR, Ramos CIV, Fateixa S, Moura NMM. Neves MGPMS, Trindade T. Hybrids based on graphene oxide and porphyrin as tools for detection and stabilization of DNA G-quadruplexes. ACS Omega. 2018;3(9):11184–91.10.1021/acsomega.8b01366Search in Google Scholar
 Zhao F, Li H, Jiang Y, Wang X, Mu X. Co-immobilization of multi-enzyme on control-reduced graphene oxide by non-covalent bonds: an artificial biocatalytic system for the one-pot production of gluconic acid from starch. Green Chem. 2014;16:2558.10.1039/c3gc42545bSearch in Google Scholar
 Jin X, Zhang H, Li Y-T, Xiao MM, Zhang ZL, Pang DW, et al. A field effect transistor modified with reduced graphene oxide for immunodetection of Ebola virus. Microchim Acta. 2019;186(4):223.10.1007/s00604-019-3256-5Search in Google Scholar PubMed
 Maity A, Sui X, Jin B, Pu H, Bottum KJ, Huang X, et al. Resonance-frequency modulation for rapid, point-of-care Ebola-glycoprotein diagnosis with a graphene-based field-effect biotransistor. Anal Chem. 2018;90(24):14230–8.10.1021/acs.analchem.8b03226Search in Google Scholar PubMed
 Thakur B, Zhou G, Chang J, Pu H, Jin B, Sui X, et al. Biosensors and bioelectronics rapid detection of single E coli bacteria using a graphene-based field-effect transistor device. Biosens Bioelectron. 2018;110:16–22.10.1016/j.bios.2018.03.014Search in Google Scholar PubMed
 Afsahi S, Lerner MB, Goldstein JM, Lee J, Tang X, Bagarozzi DA, et al. Novel graphene-based biosensor for early detection of Zika virus infection. Biosens Bioelectron. 2018;100:85–8.10.1016/j.bios.2017.08.051Search in Google Scholar PubMed
 Fan J, Yuan L, Liu Q, Tong C, Wang W, Xiao F, et al. An ultrasensitive and simple assay for the Hepatitis C virus using a reduced graphene oxide-assisted hybridization chain reaction. Analyst. 2019;144:3972–9.10.1039/C9AN00179DSearch in Google Scholar PubMed
 Li J, Li Y, Zhai X, Cao Y, Zhao J, Tang Y, et al. Sensitive electrochemical detection of hepatitis C virus subtype based on nucleotides assisted magnetic reduced graphene oxide-copper nano-composite. Electrochem Commun. 2020;110:345–58.10.1016/j.elecom.2019.106601Search in Google Scholar
 Veerapandian M, Hunter R, Neethirajan S. Dual immunosensor based on methylene blue-electroadsorbed graphene oxide for rapid detection of the influenza A virus antigen. Talanta. 2016;155:250–7.10.1016/j.talanta.2016.04.047Search in Google Scholar PubMed
 Gupta S, Kaushal A, Kumar A, Kumar D. Ultrasensitive transglutaminase based nanosensor for early detection of celiac disease in human. Int J Biol Macromol. 2017;105:905–11.10.1016/j.ijbiomac.2017.07.126Search in Google Scholar PubMed
 Islam S, Shukla S, Bajpai VK, Han YK, Huh YS, Kumar A, et al. A smart nanosensor for the detection of human immunodeficiency virus and associated cardiovascular and arthritis diseases using functionalized graphene-based transistors. Biosens Bioelectron. 2019;126:792–9.10.1016/j.bios.2018.11.041Search in Google Scholar PubMed
 Gong Q, Han H, Yang H, Zhang M, Sun X, Liang Y, et al. Sensitive electrochemical DNA sensor for the detection of HIV based on a polyaniline/graphene nanocomposite. J Mater. 2019;5:313–9.10.1016/j.jmat.2019.03.004Search in Google Scholar
 Singh M, Holzinger M, Tabrizian M, Winters S, Berner NC, Cosnier S, et al. Noncovalently functionalized monolayer graphene for sensitivity enhancement of surface plasmon resonance immunosensors. J Am Chem Soc. 2015;137:2800–3.10.1021/ja511512mSearch in Google Scholar PubMed
 Omar NAS, Fen YW, Abdullah J, Kamil YM, Daniyal WMEMM, Sadrolhosseini AR, et al. Sensitive detection of dengue virus type 2 E-proteins signals using self-assembled monolayers/reduced graphene oxide-PAMAM dendrimer thin film-SPR optical sensor. Sci Rep. 2020;10(1):2374.10.1038/s41598-020-59388-3Search in Google Scholar PubMed PubMed Central
 Kanagavalli P, Veerapandian M. Opto-electrochemical functionality of Ru(II)-reinforced graphene oxide nanosheets for immunosensing of dengue virus non-structural 1 protein. Biosens Bioelectron. 2020;150:111878.10.1016/j.bios.2019.111878Search in Google Scholar PubMed
 Abd Muain MF, Cheo KH, Omar MN, Hamzah ASA, Lim HN, Salleh AB, et al. Gold nanoparticle-decorated reduced-graphene oxide targeting anti hepatitis B virus core antigen. Bioelectrochemistry. 2018;122:199–205.10.1016/j.bioelechem.2018.04.004Search in Google Scholar PubMed
 Xiang Q, Huang J, Huang H, Mao W, Ye Z. A label-free electrochemical platform for the highly sensitive detection of hepatitis B virus DNA using graphene quantum dots. RSC Adv. 2018;8:1820–5.10.1039/C7RA11945CSearch in Google Scholar PubMed PubMed Central
 Ahmed SR, Mogus J, Chand R, Nagy E, Neethirajan S. Optoelectronic fowl adenovirus detection based on local electric field enhancement on graphene quantum dots and gold nanobundle hybrid. Biosens Bioelectron. 2018;103:45–53.10.1016/j.bios.2017.12.028Search in Google Scholar PubMed
 Farzin L, Sadjadi S, Shamsipur M, Sheibani S. Electrochemical genosensor based on carbon nanotube/amine-ionic liquid functionalized reduced graphene oxide nanoplatform for detection of human papillomavirus (HPV16)-related head and neck cancer. J Pharm Biomed Anal. 2020;179:112989.10.1016/j.jpba.2019.112989Search in Google Scholar PubMed
 Li J, Li Y, Zhai X, Cao Y, Zhao J, Tang Y, et al. Sensitive electrochemical detection of hepatitis C virus subtype based on nucleotides assisted magnetic reduced graphene oxide-copper nano-composite. Electrochem Commun. 2020;110:106601.10.1016/j.elecom.2019.106601Search in Google Scholar
 Jaiswal N, Pandey CM, Solanki S, Tiwari I, Malhotra BD. An impedimetric biosensor based on electrophoretically assembled ZnO nanorods and carboxylated graphene nanoflakes on an indium tin oxide electrode for detection of the DNA of Escherichia coli O157:H7. Microchim Acta. 2020;187:1.10.1007/s00604-019-3921-8Search in Google Scholar PubMed
 Zi´ołkowski R, Oszwałdowski S, Kopyra KK, Zacharczuk K, Zasada AA, Malinowska E. Toward fluorimetric-paired-emitter-detector-diode test for Bacillus anthracis DNA based on graphene oxide. Microchem J. 2020;154:104592.10.1016/j.microc.2019.104592Search in Google Scholar
 Ji J, Pang Y, Li D, Wang X, Xu Y, Mu X. Single-layered graphene/Au-nanoparticles-based love wave biosensor for highly sensitive and specific detection of Staphylococcus aureus gene sequences. ACS Appl Mater Interfaces. 2020;12:12417–25.10.1021/acsami.9b20639Search in Google Scholar PubMed
 Li X, Wang Y, Zhang X, Gao Y, Sun C, Ding Y, et al. An impedimetric immunosensor for determination of porcine epidemic diarrhea virus based on the nanocomposite consisting of molybdenum disulfide/reduced graphene oxide decorated with gold nanoparticles. Microchim Acta. 2020;187:217.10.1007/s00604-020-4166-2Search in Google Scholar PubMed
 You Z, Qiu Q, Chen H, Feng Y, Wang X, Wang Y, et al. Laser-induced noble metal nanoparticle-graphene composites enabled flexible biosensor for pathogen detection. Biosens Bioelectron. 2020;150:111896.10.1016/j.bios.2019.111896Search in Google Scholar PubMed
 Zhao W, Xing Y, Lin Y, Gao Y, Wu M, Xu J. Monolayer graphene chemiresistive biosensor for rapid bacteria detection in a microchannel. Sens Actuators Rep. 2020;2:100004.10.1016/j.snr.2020.100004Search in Google Scholar
 Pang S, Gao Y, Li Y, Liu S, Su X. A novel sensing strategy for the detection of Staphylococcus aureus DNA by using a graphene oxide-based fluorescent probe. Analyst. 2013;138:2749–54.10.1039/c3an36642aSearch in Google Scholar PubMed
 Qaddare SH, Salimi A. Amplified fluorescent sensing of DNA using luminescent carbon dots and AuNPs/GO as a sensing platform: a novel coupling of FRET and DNA hybridization for homogeneous HIV-1 gene detection at femtomolar level. Biosens Bioelectron. 2017;89:773–80.10.1016/j.bios.2016.10.033Search in Google Scholar PubMed
 He S, Song B, Li D, Zhu C, Qi W, Wen Y, et al. A graphene nanoprobe for rapid, sensitive, and multicolor fluorescent DNA analysis. Adv Funct Mater. 2010;20:453–9.10.1002/adfm.200901639Search in Google Scholar
 Liu C, Wang Z, Jia H, Li Z. Efficient fluorescence resonance energy transfer between upconversion nanophosphors and graphene oxide: a highly sensitive biosensing platform. Chem Commun. 2011;47:4661–3.10.1039/c1cc10597cSearch in Google Scholar PubMed
 Liu F, Choi JY, Seo TS. Graphene oxide arrays for detecting specific DNA hybridization by fluorescence resonance energy transfer. Biosens Bioelectron. 2010;25:2361–5.10.1016/j.bios.2010.02.022Search in Google Scholar PubMed
 Jiang Y, Tian J, Chen S, Zhao Y, Wang Y, Zhao S. A graphene oxide-based sensing platform for the label-free assay of DNA sequence and exonuclease activity via long range resonance energy transfer. J Fluoresc. 2013;23:697–703.10.1007/s10895-013-1189-7Search in Google Scholar PubMed
 Benvidi A, Rajabzadeh N, Mazloum-Ardakani M, Heidari MM, Mulchandani A. Simple and label-free electrochemical impedance amelogenin gene hybridization biosensing based on reduced graphene oxide. Biosens Bioelectron. 2014;58:145–52.10.1016/j.bios.2014.01.053Search in Google Scholar PubMed
 Mihrican M, Surbhi S, Arzum E, Pagona P. Electrochemical monitoring of nucleic acid hybridization by single-use graphene oxide-based sensor. Electroanalysis. 2011;23:272–9.10.1002/elan.201000425Search in Google Scholar
 Ye Y, Xie J, Ye Y, Cao X, Zheng H, Xu X, et al. A label-free electrochemical DNA biosensor based on thionine functionalized reduced graphene oxide. Carbon. 2018;129:730–7.10.1016/j.carbon.2017.12.060Search in Google Scholar
 Li B, Pan G, Avent ND, Lowry RB, Madgett TE, Waines PL. Graphene electrode modified with electrochemically reduced graphene oxide for label-free DNA detection. Biosens Bioelectron. 2015;72:313–9.10.1016/j.bios.2015.05.034Search in Google Scholar PubMed
 Hwang MT, Heiranian M, Kim Y, You S, Leem J, Taqieddin A, et al. Ultrasensitive detection of nucleic acids using deformed graphene channel field effect biosensors. Nat Commun. 2020;11:1–11.10.1038/s41467-020-15330-9Search in Google Scholar PubMed PubMed Central
 Tian M, Xu S, Zhang J, Wang X, Li Z, Liu H, et al. RNA detection based on graphene field-effect transistor biosensor. Adv Condens Matter Phys. 2018;2018:8146765.10.1155/2018/8146765Search in Google Scholar
 Hwang MT, Heiranian M, Kim Y, You S, Leem J, Taqieddin A, et al. Ultrasensitive detection of nucleic acids using deformed graphene channel field effect biosensors. Nat Comm. 2020;11:1543.10.1038/s41467-020-15330-9Search in Google Scholar
 Bagherzadeh-Nobari S, Kalantarinejad R. Real-time label-free detection of DNA hybridization using a functionalized graphene field effect transistor: a theoretical study. J Nanopart Res. 2021;23:185.10.1007/s11051-021-05295-1Search in Google Scholar PubMed PubMed Central
 Chen Z, Liu X, Liu D, Li F, Wang L, Liu S. Ultrasensitive electrochemical DNA biosensor fabrication by coupling an integral multifunctional zirconia-reduced graphene oxide-Tthionine nanocomposite and exonuclease I-assisted cleavage. Front Chem. 2020;8:521.10.3389/fchem.2020.00521Search in Google Scholar PubMed PubMed Central
 Povedano E, Cincotto FH, Parrado C, Díez P, Sánchez A, Canevari TC, et al. Decoration of reduced graphene oxide with rhodium nanoparticles for the design of a sensitive electrochemical enzyme biosensor for 17β-estradiol. Biosens Bioelectron. 2017;89:343–51.10.1016/j.bios.2016.07.018Search in Google Scholar PubMed
 Palanisamy S, Ramaraj SK, Chen S-M, Yang TCK, Yi-Fan P, Chen T-W, et al. A novel laccase biosensor based on laccase immobilized graphene–cellulose microfiber composite modified screen-printed carbon electrode for sensitive determination of catechol. Sci Rep. 2017;7:41214.10.1038/srep41214Search in Google Scholar PubMed PubMed Central
 Liu J, Wang T, Wang J, Wang E. Mussel-inspired biopolymer modified 3D graphene foam for enzyme immobilization and high performance biosensor. Electrochim Acta. 2015;161:17–22.10.1016/j.electacta.2015.02.034Search in Google Scholar
 Fan Z, Lin Q, Gong P, Liu B, Wang J, Yang S. A new enzymatic immobilization carrier based on graphene capsule for hydrogen peroxide biosensors. Electrochim Acta. 2015;151:186–94.10.1016/j.electacta.2014.11.022Search in Google Scholar
 Vasilescu I, Eremia SAV, Kusko M, Radoi A, Vasile E, Radu G-L. Molybdenum disulphide and graphene quantum dots as electrode modifiers for laccase biosensor. Biosens Bioelectron. 2016;75:232–7.10.1016/j.bios.2015.08.051Search in Google Scholar PubMed
 Mansouri N, Babadi AA, Bagheri S, Hamid SBA. Immobilization of glucose oxidase on 3D graphene thin film: novel glucose bioanalytical sensing platform. Int J Hydrog Energy. 2017;42:1337–43.10.1016/j.ijhydene.2016.10.002Search in Google Scholar
 Kang Z, Jiao K, Xu X, Peng R, Jiao S, Hu Z. Graphene oxide-supported carbon nanofiber-like network derived from polyaniline: a novel composite for enhanced glucose oxidase bioelectrode performance. Biosens Bioelectron. 2017;96:367–72.10.1016/j.bios.2017.05.025Search in Google Scholar PubMed
 Chuck A, Kim HE, Moreira JK, Lora PS, Kim YS. A graphene-based enzymatic biosensor using a common-gate field-effect transistor for L-lactic acid detection in blood plasma samples. Sens (Basel). 2021;21(5):1852.10.3390/s21051852Search in Google Scholar PubMed PubMed Central
 Luo Y, Zhang Y, Lu L, Luo H. A flexible CVD graphene platform electrode modified with l-aspartic acid for the simultaneous determination of acetaminophen, epinephrine and tyrosine. J Electroanal Chem. 2020;856:113737.10.1016/j.jelechem.2019.113737Search in Google Scholar
 Chauhan D, Nohwal B, Pundir C. An electrochemical CD59 targeted noninvasive immunosensor based on graphene oxide nanoparticles embodied pencil graphite for detection of lung cancer. Microchem J. 2020;156:104957.10.1016/j.microc.2020.104957Search in Google Scholar
 Wei S, Hao Y, Ying Z, Xu C, Wei Q, Xue S, et al. Transfer-free CVD graphene for highly sensitive glucose sensors. J Mater Sci Technol. 2020;37:71–6.10.1016/j.jmst.2019.07.039Search in Google Scholar
 Alafeef M, Dighe K, Moitra P, Pan D. Rapid, ultrasensitive, and quantitative detection of SARS-CoV-2 using antisense oligonucleotides directed electrochemical biosensor chip. ACS Nano. 2020;14(12):17028–45.10.1021/acsnano.0c06392Search in Google Scholar PubMed PubMed Central
 Torrente-Rodríguez RM, Lukas H, Tu J, Min J, Yang Y, Xu C, et al. SARS-CoV-2 RapidPlex: a graphene-based multiplexed telemedicine platform for rapid and low-cost COVID-19 diagnosis and monitoring. Matter. 2020;3(6):1981–98.10.1016/j.matt.2020.09.027Search in Google Scholar PubMed PubMed Central
 Srivastava AK, Dwivedi N, Dhand C, Khan R, Sathish N, Gupta MK, et al. Potential of graphene-based materials to combat COVID-19: properties, perspectives, and prospects. Mater Today Chem. 2020;18:100385.10.1016/j.mtchem.2020.100385Search in Google Scholar PubMed PubMed Central
 Abid SA, Muneer AA, Al-Kadmy IMS, Sattar AA, Beshbishy AM, Batiha GS, et al. Biosensors as a future diagnostic approach for COVID-19. Life Sci. 2021;273:119117.10.1016/j.lfs.2021.119117Search in Google Scholar PubMed PubMed Central
 Sadat S, Sarah M, Flynn E, Mahshid S. The potential application of electrochemical biosensors in the COVID-19 pandemic: a perspective on the rapid diagnostics of SARS-CoV-2. Biosens Bioelectron. 2021;176:112905.10.1016/j.bios.2020.112905Search in Google Scholar PubMed PubMed Central
 Sengupta J, Hussain CM. Graphene-based field-effect transistor biosensors for the rapid detection and analysis of viruses: a perspective in view of COVID-19. Carbon Trends. 2021;2:100011.10.1016/j.cartre.2020.100011Search in Google Scholar
 Seo G, Lee G, Kim MJ, Baek S-H, Choi M, Ku KB, et al. Rapid detection of COVID-19 causative virus (SARS-CoV-2) in human nasopharyngeal swab specimens using field-effect transistor-based biosensor. ACS Nano. 2020; 14(4):5135–42.10.1021/acsnano.0c02823Search in Google Scholar PubMed PubMed Central
 Mavrikou S, Moschopoulou G, Tsekouras V, Kintzios S. Development of a portable, ultra-rapid and ultra-sensitive cell-based biosensor for the direct detection of the SARS-CoV-2 S1 spike protein antigen. Sens (Basel). 2020;20(11):3121.10.3390/s20113121Search in Google Scholar PubMed PubMed Central
 Huang Z, Tian D, Liu Y, Lin Z, Lyon CJ, Lai W, et al. Ultra-sensitive and high-throughput CRISPR-powered COVID-19 diagnosis. Biosens Bioelectron. 2020;164:112316.10.1016/j.bios.2020.112316Search in Google Scholar PubMed PubMed Central
 Li J, Lillehoj PB. Microfluidic magneto immunosensor for rapid, high sensitivity measurements of SARS-CoV-2 nucleocapsid protein in serum. ACS Sens. 2021;6(3):1270–8.10.1021/acssensors.0c02561Search in Google Scholar PubMed PubMed Central
 Zhao H, Liu F, Xie W, Zhou T-C, Yang JO, Jin L, et al. Ultrasensitive supersandwich-type electrochemical sensor for SARS-CoV-2 from the infected COVID-19 patients using a smartphone. Sens Actuators B Chem. 2021;327:128899.10.1016/j.snb.2020.128899Search in Google Scholar PubMed PubMed Central
 Fabiani L, Saroglia M, Galatà G, De Santis R, Fillo S, Luca V, et al. Magnetic beads combined with carbon black-based screen-printed electrodes for COVID-19: a reliable and miniaturized electrochemical immunosensor for SARS-CoV-2 detection in saliva. Biosens Bioelectron. 2021;171:112686.10.1016/j.bios.2020.112686Search in Google Scholar PubMed PubMed Central
 Farzin L, Sadjadi S, Sheini A, Mohagheghpour E. A nanoscale genosensor for early detection of COVID-19 by voltammetric determination of RNA-dependent RNA polymerase (RdRP) sequence of SARS-CoV-2 virus. Microchim Acta. 2021;188(4):121.10.1007/s00604-021-04773-6Search in Google Scholar PubMed PubMed Central
 Yakoha A, Pimpitaka U, Rengpipat S, Hirankarnd N, Chailapakul O, Chaiyoa S. Paper-based electrochemical biosensor for diagnosing COVID-19: detection of SARS-CoV-2 antibodies and antigen. Biosens Bioelectron. 2021;176:112912.10.1016/j.bios.2020.112912Search in Google Scholar PubMed PubMed Central
 Ke G, Su D, Li Y, Zhao Y, Wang H, Liu W, et al. An accurate, high-speed, portable bifunctional electrical detector for COVID-19. Sci China Mat. 2021;64:739–47.10.1007/s40843-020-1577-ySearch in Google Scholar PubMed PubMed Central
 Bouchiat V, Girit C, Kessler B, Zettl AK. Graphene device and method of using graphene device. US9105793B2; 2010.Search in Google Scholar
 James O. Guy graphene biosensor. WO2011004136A1; 2011.Search in Google Scholar
 Cui Y. Flexible Graphene Biosensor. US20130248380A1; 2013. Utah State University USU (current assignee).Search in Google Scholar
 Mohapatra SS, Cissell KA, Alwarappan S. Chitosan-graphene biosensors and methods for their use. US9091640B1; 2013.Search in Google Scholar
 Nowak C. Graphene FET-based biosensor. EP2848929A1. European Patent Office. AIT Austrian Institute of Technology GmbH (current assignee); 2013.Search in Google Scholar
 Okai M. Graphene sensor, substance species analyzer using sensor, and method for detecting substance species using sensor. JP2012247189A; 2014.Search in Google Scholar
 Roy S, Rahman IA, Ahmed MU. Novel electrochemical DNA biosensor using graphene biochip for species identification. US20160177387A1; 2015.Search in Google Scholar
 Shicai X, Meng T, Jihua W, Guodong H, Ruihong S. Method for detecting guanine ribose switch affinity based on graphene biosensor. CN109358103B; 2018.Search in Google Scholar
 Shicai X, Ruihong S, Chonghui L, Jihua W, Meng T, Yingxian L. Method for detecting cancer marker MicroRNA based on three-dimensional graphene biosensor. CN110699431A; 2019.Search in Google Scholar
 Teng KS, Deganello D, Samavat S, Zhang W. Graphene biosensor and process of manufacture. WO2021001231A1; 2019.Search in Google Scholar
 He B. Xinhua Hospital, Shanghai Jiao Tong University School of Medicine, Clinical Trails of Photoelectrochemical Immunosensor for Early Diagnosis of Acute Myocardial Infarction, ClinicalTrials.gov Identifier: NCT04390490.Search in Google Scholar
 Kala D, Sharma TK, Gupta S, Verma V, Thakur A, Kaushal A, et al. Graphene oxide nanoparticles modified paper electrode as a biosensing platform for detection of the htrA gene of O. tsutsugamushi. Sens (Basel). 2021;21(13):4366.10.3390/s21134366Search in Google Scholar PubMed PubMed Central
 Furion analytics Research & Consulting LLP, Biomedical Sensor Market – Forecast (2021–2026), Available from: https://www.industryarc.com/Report/1315/bio-medical-sensor-market.html (accessed May 17, 2021).Search in Google Scholar
 TechVision Group, Frost and Sullivan, Key opportunities and trends in biosensors. 2018–2023, Conference Proceedings, International Micro Nano conference, Amsterdam, December 11–12, 2018. Available from: https://fhi.nl/app/uploads/sites/57/2018/12/Micro-Nano-Slides-December-8-2018-Final.pdf (accessed May 17, 2021)Search in Google Scholar
 Collins R. Graphene market and 2D materials assessment 2021–2031. Available from: www.idtechex.com (accessed May 17, 2021).Search in Google Scholar
 The ARC graphene research hub for Graphene Enabled Industry Transformation, The University of Adelaide, Available from: https://arcgrapheneresearchhub.com.au/ (accessed May 17, 2021).Search in Google Scholar
 Pomager J. Graphene Biosensors. The next frontier in medical diagnostics; 2014. Available from: www.meddeviceonline.com (accessed May 17, 2021).Search in Google Scholar
 Goldsmith BR, Locascio L, Gao Y, Lerner M, Walker A, Lerner J, et al. Digital biosensing by Foundry-fabricated graphene sensors. Sci Rep. 2019;9:434.10.1038/s41598-019-38700-wSearch in Google Scholar PubMed PubMed Central
 Ye S, Feng S, Huang L, Bian S. Recent progress in wearable biosensors: from healthcare monitoring to sports analytics. Biosens (Basel). 2020;10(12):205.10.3390/bios10120205Search in Google Scholar PubMed PubMed Central
 Mathew M, Radhakrishnan S, Vaidyanathan A, Chakraborty B, Rout CS. Flexible and wearable electrochemical biosensors based on two-dimensional materials: recent developments. Anal Bioanal Chem. 2021;413(3):727–62.10.1007/s00216-020-03002-ySearch in Google Scholar PubMed PubMed Central
 Sharma A, Badea M, Tiwari S, Marty JL. Wearable biosensors: an alternative and practical approach in healthcare and disease monitoring. Molecules. 2021;26(3):748.10.3390/molecules26030748Search in Google Scholar PubMed PubMed Central
© 2022 Hassan A. Alhazmi et al., published by De Gruyter
This work is licensed under the Creative Commons Attribution 4.0 International License.